Analgsis of
Composite tructures
This Page Intentionally Left Blank
Analysis of
Composite Structures
Christian De...
844 downloads
2430 Views
8MB Size
Report
This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!
Report copyright / DMCA form
Analgsis of
Composite tructures
This Page Intentionally Left Blank
Analysis of
Composite Structures
Christian Decolon
First published in 2000 by Hermes Science Publications, Paris First published in English in 2002 by Hermes Penton Ltd Apart from any fair dealing for the purposes of research or private study, or criticism or review, as permitted under the Copyright, Designs and Patents Act 1988, this publication may only be reproduced, stored or transmitted, in any form or by any means, with the prior permission in writing of the publishers, or in the case of reprographic reproduction in accordance with the terms and licences issued by the CLA. Enquiries concerning reproduction outside these terms should be sent to the publishers at the undermentioned address: Hermes Penton Science 120 Pentonville Road London N 1 9JN 9Hermes Science Publications, 2000 9English language edition, Hermes Penton Ltd, 2002 The right of Christian Decolon to be identified as the author of this work has been asserted by him in accordance with the Copyright, Designs and Patents Act 1988.
British Library Cataloguing in Publication Data A CIP record for this book is available from the British Library. ISBN 1 9039 9602 3
Transferred to digital printing 2006
Contents
Foreword ................................................................................................................ xiii PART I
1.
Constitutive relations for anisotroptc materials in linear elasticity ............. 3 1.1. 1.2.
1.3. 1.4.
1.5.
2.
Mechanical behaviour of composite materials
Introduction ............................................................................................. Four indices tensor notation .................................................................... 1.2.1. Constitutive relations ................................................................ 1.2.2. Properties of Cqt t and Sqk t ......................................................
3 3 3 4
Conventional two indices Voigt notation ................................................ 5 Anisotropic material ................................................................................ 6 1.4.1. Monoclinic material .................................................................. 6 1.4.2. Orthotropic material .................................................................. 9 1.4.3. Transversely isotropic material ............................................... 14 1.4.4. Isotropic material .................................................................... 17 1.4.5. Influence of temperature and humidity on the constitutive relation of an orthotropic material ............ 19 Matrix relations for a change of axes .................................................... 20 1.5.1. Change of axes for stress and strain matrices ......................... 20 1.5.2. Change of axes for stiffness and compliance matrices ............ 24
Orthotropic layer behavlour ......................................................................... 25 2.1. 2.2. 2.3.
Introduction ........................................................................................... 25 Stiffness and compliance matrices in orthotropic coordinates ............. 25 Conventional matrices for changing axes ............................................. 27
vi
Contents
2.4. 2.5. 2.6. 2.7.
2.8.
2.9.
3.
29 30 32 35 35 37 38
2.8.1.
Reduced stiffness matrix Q in orthotropic coordinates ........ 38
2.8.2.
Reduced stiffness matrix Q in the coordinates
away from the orthotropic axes ............................................... Reduced compliance matrices of an orthotropic layer .......................... 2.9.1. Reduced compliance matrix in orthotropic coordinates ......... 2.9.2. Reduced compliance matrix P in the direction away from the orthotropic axes ...............................................
40 43 43 43
Elastic constants of a unidirectional c o m p o s i t e ........................................... 45
3.1.
4.
Stress and strain matrices ...................................................................... Stiffness matrix in directions away from the orthotropic axes .............. Compliance matrix in directions away from the orthotropic axes ......... Orthotropic layer loaded in tension and in shear ................................... 2.7.1. Simple tension ........................................................................... 2.7.2. Simple shear ............................................................................... Reduced stiffness matrix for the orthotropic layer ................................
3.2.
Introduction ........................................................................................... 45 Density p ............................................................................................. 45
3.3.
Longitudinal Young's modulus E l ....................................................... 46
3.4.
Poisson's coefficient v12 ........................................................................ 47
3.5.
Transverse Young's modulus E 2 .......................................................... 48
3.6.
Shear modulus Gl2 ............................................................................... 49
3.7.
Longitudinal thermal expansion coefficient ct I .................................... 51
3.8.
Transverse expansion coefficient ct 2 ................................................... 52
Failure
4.1. 4.2. 4.3. 4.4.
4.5.
4.6.
criteria
................................................................................................
Introduction ........................................................................................... Maximum stress theory ......................................................................... Maximum strain theory ......................................................................... Polynomial failure criteria .................................................................... 4.4.1. TsaiHill criterion .................................................................... 4.4.2. TsaiWu criterion .................................................................... 4.4.3. Hoffman criterion .................................................................... Tensile and shear strength of a unidirectional layer .............................. 4.5.1. Tensile strength ....................................................................... 4.5.2. Shear strength .......................................................................... Determination of failure stresses from three tension tests .....................
55
55 55 56 57 57 60 62 64 64 67 70
Contents PART II
5.
Multilayer plates
Multilayer KirchhoffLove thin plates ........................................................ 73 5.1. 5.2. 5.3. 5.4. 5.5.
Introduction ........................................................................................... KirchhoffLove hypotheses for thin plates ............................................ Straindisplacement relationships ......................................................... Global plate equations ........................................................................... Calculation of I 0 ..................................................................................
73 73 74 75 76
5.6. 5.7. 5.8. 5.9.
Stress field ............................................................................................. Global cohesive forces .......................................................................... Composite global stiffness matrix ......................................................... Decoupling ............................................................................................ 5.9.1. Membraneflexion decoupling ................................................ 5.9.2. Tensionshear decoupling ....................................................... 5.9.3. Membraneflexion and tensionshear decoupling ................... Global stiffnesses of a symmetrical composite ..................................... 5.10.1. Symmetrical laminate (a',fl)Ns ..............................................
77 77 78 79 79 80 82 82 82
5 10.2. 9
Symmetrical crossply laminate (0, a) 2 NS
85
5.10.3.
Symmetrical balanced laminate (a,a,)N s ............................. 86
5.10.
5.11.
5.12.
5.13.
5.14. 5.15.
6.
vii
...............................
Global stiffnesses for an asymmetrical laminate ................................... 87 5.11.1. Asymmetrical laminate (a,,B)N .............................................. 87 5. 1 1.2.
Asymmetrical crossply laminate (0,ff)N ............................... 90
5.11.3.
Asymmetrical balanced laminate (ct,ct)N ............................ 91
Examples of global stiffness matrices ................................................... 91 5.12. I. Two layer plate ....................................................................... 91 5.12.2. Three layer plate ..................................................................... 92 5.12.3. Four layer plate ....................................................................... 93 5.12.4. Examples of decoupling .......................................................... 93 Boundary conditions ............................................................................. 95 5.13. I. Definition of boundary conditions .......................................... 95 5.13.2. Effective global transverse shear load ..................................... 96 Determination of transverse shear stresses .......................................... 100 Strain energy ....................................................................................... 103
Symmetrical orthotroplc KlrchhoffLove plates ....................................... 105 6.1.
6.2.
Introduction ......................................................................................... Global plate equations .........................................................................
105 106
viii
Contents
6.3. 6.4. 6.5. 6.6. 6.7.
Plate loaded in the mean plane ............................................................ Plate loaded transversely ..................................................................... Flexure of a rectangular plate simply supported around its edge ........ Free vibrations of a rectangular plate freely supported at its edge ...... Buckling of a rectangular plate simply supported at its edge .............. 6.7.1. General case .......................................................................... 6.7.2. Case of k  0 ....................................................................... 6.7.3. Case of k = 1 ........................................................................ 6.7.4.
7.
121
121 123 127
Case of k =  1 / 2 .................................................................. 128
Thermoelastic behaviour of composites .................................................... 131
7.1. 7.2.
7.3.
7.4. 7.5. 7.6.
7.7.
8.
106 107 109 118
Introduction ......................................................................................... Constitutive relation for an orthotropic material ................................. 7.2.1. Constitutive relation in orthotropic axes ............................... 7.2.2. Constitutive relation in orthotropic offaxes ......................... Constitutive relation when the normal transverse stress is zero .......... 7.3.1. Constitutive relation in orthotropic axes ............................... 7.3.2. Constitutive relation in orthotropic offaxes ......................... Global cohesion forces ........................................................................ Global composite constitutive relation ................................................ Decoupling .......................................................................................... 7.6.1. Composite with mirror s y m m e t r y ......................................... 7.6.2. Balanced composite .............................................................. 7.6.3. Balanced symmetrical composite .......................................... Balanced symmetrical composite loaded in the mean plane ...............
131 131
131 133 135 135 135 136 137 138 138 138 139 139
Symmetrical orthotropic ReissnerMindlin plates .................................... 141
8.1. 8.2. 8.3. 8.4. 8.5. 8.6. 8.7. 8.8.
8.9. 8.10.
Introduction ......................................................................................... Moderately thick plate, ReissnerMindlin assumptions ...................... Displacements, strains and stresses ..................................................... Global plate equations ......................................................................... Calculation of I I and 12 .....................................................................
141 141
Global cohesive forces ........................................................................ Global stiffness matrix of the c o m p o s i t e ............................................. Transverse shear correction coefficient ............................................... 8.8.1. Uflyand coefficient ............................................................... 8.8.2. Reissner coefficient ............................................................... Boundary conditions ........................................................................... Symmetrical orthotropic plate .............................................................
143 144 145 145 147 149 149
14 l 142 142
Contents 8.11. 8.12. 8.13.
0
Flexure of a rectangular orthotropic symmetrical plate simply supported around its edge ........................................................ 150 Transverse vibration of a rectangular orthotropic symmetrical plate simply supported around its edge ............................................... 153 Buckling of a rectangular orthotropic symmetrical plate simply supported around its edge ............................................... 155
Asymmetrical multilayer Kirchhoff.Love plates .................................................................................. 159 9.1. 9.2. 9.3. 9.4. 9.5. 9.6. 9.7.
10.
ix
Introduction ......................................................................................... Flexure of a crossply asymmetrical plate ........................................... Vibration of an crossply asymmetrical plate ...................................... Buckling of a crossply asymmetrical plate ........................................ Flexure of a balanced asymmetrical plate ........................................... Vibration of a balanced asymmetrical plate ........................................ Buckling of a balanced asymmetrical plate .........................................
Cylindrical flexure of multilayer Kirchhoff.Love plates .................................................................................. 10.1. 10.2. 10.3. 10.4. 10.5.
10.6.
159 159 165 170 175 182 189
195
Introduction ......................................................................................... Straindisplacement relationship ......................................................... Global constitutive relation ................................................................. Global plate equations ......................................................................... Flexure ................................................................................................ 10.5.1. Elimination of u~ and u~ ....................................................
195 195 196 197 198 199
10.5.2. Simply supported plate subjected to a sinusoidal load .......... Vibrations ............................................................................................ 10.6.1. General case .......................................................................... 10.6.2. Asymmetrical crossply composite (O,~)N..........................
200 204 204 206
10.6.3.
Balanced asymmetrical composite (Ot,Ot)N ........................
10.6.4. Symmetrical composite ......................................................... 10.7. Buckling .............................................................................................. I0.7.1. General case .......................................................................... 10.7.2. Crossply asymmetrical composite (0,~)N...........................
208 209 211 211 214
10.7.3.
Balanced asymmetrical composite (Ct,Ct)N ........................ 214
10.7.4.
Symmetrical composite ......................................................... 214
x
11.
Contents
Cylindrical flexure of multilayer ReissnerMindlin plates ............................................................................... 215 11.1. 11.2. 11.3. 11.4. 11.5. 11.6. 11.7.
PART III
12.
Multilayer beams
Introduction ......................................................................................... Strains, stresses, global equation of tensioncompression ................... Single layer orthotropic beam ............................................................. General equations for beams in tensioncompression ......................... Builtin beam under its own weight and subjected to a force ............. Vibration of a builtin beam ................................................................
231 231 233 234 235 237
Symmetrical multilayer beams in flexure without transverse shear strain ................................................................... 239 13.1. 13.2. 13.3. 13.4.
Introduction ......................................................................................... Strains, stresses, equations of motion .................................................. Monolayer orthotropic beam ............................................................... General beam equations ...................................................................... 13.4.1. Flexure in the plane (Olx 2, x3) ............................................. 13.4.2.
13.5. 13.6. 13.7.
14.
215 215 215 216 218 222 225
Symmetrical multilayer beams in tensioncompression .......................... 231 12.1. 12.2. 12.3. 12.4. 12.5. 12.6.
13.
Introduction ......................................................................................... Straindisplacement relationship ......................................................... Global constitutive relation ................................................................. Global plate equations ......................................................................... Flexure ................................................................................................. Vibrations ............................................................................................ Buckling ..............................................................................................
239 239 243 244 244
Flexure in the plane (Olx l , x 2) ............................................. 247
Simply supported beam subjected to sinusoidal loads ........................ 249 Vibrations of a simply supported beam ............................................... 250 Buckling of a simply supported beam ................................................. 251
Symmetrical multilayer beams in flexure with transverse shear strain ........................................................................ 253 14.1. 14.2. 14.3. 14.4.
Introduction ......................................................................................... Strains, stresses, global equations ....................................................... Monolayer orthotropic beam ............................................................... General beam equations ......................................................................
253 253 256 258
Contents
14.5. 14.6. 14.7.
/
,
xi
\
14.4.1.
Flexure in the plane I,Olxl,x3) ............................................. 258
14.4.2.
Flexure in the plane (Olxl, x 2 ) ............................................. 260
Simply supported beam subjected to a sinusoidal load ....................... 261 Vibration of a simply supported beam ................................................ 263 Buckling of a simply supported beam ................................................. 266
APPENDICES Global plate equations
15.
Global plate equations neglecting large transverse displacements .................................................................... 271 15.1. 15.2. 15.3. 15.4.
15.5.
15.6.
16.
Introduction ......................................................................................... Hypothesis relating to plates ............................................................... ReissnerMindlin and KirchhoffLove plates theories ........................ Global plate equations ......................................................................... 15.4.1. Force equations ..................................................................... 15.4.2. Moment equations ................................................................. Plate equations in ReissnerMindlin analysis ...................................... 15.5.1. Calculation of second members ............................................ 15.5.2. Global plate equations ........................................................... 15.5.3. Boundary conditions ............................................................. Plate equations in KirchhoffLove analysis ........................................ 15.6.1. Calculation of second members ............................................ 15.6.2. Global plate equations ........................................................... 15.6.3. Boundary edge conditions ......................... "...........................
271 271 272 278 278 280 281 281 282 283 283 283 284 285
Global plate equations for large transverse displacements ...................... 287 16.1. 16.2. 16.3.
16.4.
16.5. 16.6.
Introduction ......................................................................................... Local plate equations .......................................................................... Global plate equations ......................................................................... 16.3.1. Global plate summation equations ........................................ 16.3.2. Global plate moment equations ............................................. Global plate equations for static, vibration and buckling cases .......... 16.4.1. Global plate equations ........................................................... 16.4.2. Global plate equilibrium equations ....................................... 16.4.3. Global plate vibration equations ........................................... 16.4.4. Global plate buckling equations ............................................ ReissnerMindlin global plate equations ............................................. KirchhoffLove global plate equations ...............................................
287 287 288 288 291 293 293 293 294 295 295 296
xii
Contents
17.
Global plate equations: KirchhoffLove theory v a r i a t i o n a l f o r m u l a t i o n ................................................................................ 297 17.1. 17.2. 17.3.
17.4.
17.5.
18.
Introduction ......................................................................................... Von Karman strains ............................................................................ Variational formulation ....................................................................... 17.3.1. Virtual work of internal forces .............................................. 17.3.2. Virtual work of transverse surface forces ............................. 17.3.3. Virtual work of external lateral surface forces ...................... 17.3.4. Virtual work of body forces .................................................. 17.3.5. Virtual work done by inertial forces ..................................... 17.3.6. Variational formulation ......................................................... Global plate equations, boundary edge conditions .............................. 17.4.1. Global plate equations ........................................................... 17.4.2. Boundary edge conditions ..................................................... Global plate equations in static, vibration and buckling cases ............
Global plate equations: ReissnerMindlin theory variational formulation ................................................................................ 18.1. 18.2. 18.3.
18.4.
18.5.
Introduction ......................................................................................... Von Karman strains ............................................................................ Variational formulation ....................................................................... 18.3.1. Virtual work of internal forces .............................................. 18.3.2. Virtual work of transverse surface forces ............................. 18.3.3. Virtual work of external lateral surface forces ...................... 18.3.4. Virtual work of body forces .................................................. 18.3.5. Virtual work done by inertial forces ..................................... 18.3.6. Variational formulation ......................................................... Global equations, boundary edge conditions ...................................... 18.4.1. Global plate equations ........................................................... 18.4.2. Boundary edge conditions ..................................................... Global static, vibration and buckling equations ..................................
References ..............................................................................................................
297 297 301 301 304 304 305 306 307 308 308 309 313
315 315 315 316 317 320 320 320 321 322 323 323 325 328
331
I n d e x ...................................................................................................................... 333
Foreword
The aim of this book is to present the basis for calculation of composite structures, using continuum mechanics equations which enable the more elaborate theories to be treated. The first part is devoted to study of materials constituting the layers of laminated composites. The constitutive equations for anisotropic and in particular orthotropic materials are presented, with temperature and hygrometry effects taken into account. Next the basic laws of mixtures are given, which enable the behaviour of unidirectional layers to be predicted from the characteristics of their fibres and matrix components. The subject of the second part is multilayer plates. We begin by presenting the general equations of thin plates in KirchhoffLove analysis. Later, symmetrical orthotropic plates are studied in detail for cases of bending, vibration and buckling. The thermoelastic behaviour of multilayers plates is considered separately. Then we tackle symmetric orthotropic moderately thick plates, using ReissnerMindlin type analysis. Examples of asymmetrical plates in KirchhoffLove theory are analysed in detail. The cylindrical bending of laminated composites is treated in both KirchhoffLove and ReissnerMindlin type analysis, with bending, vibration and buckling applications. The third part of this book is devoted to beams. The first chapter of this part treats tensioncompression loading. The following chapter treats bending with transverse shear deformations not taken in account. The last chapter of this part presents bending taking into account transverse shear. Examples of bending, vibration and buckling are considered for each case. In the appendices, plate equations are developed by integrating local equations of motion. Global equations are obtained from variational formulae of continuum mechanics.
This Page Intentionally Left Blank
PART I
Mechanical Behaviour of Composite Materials
This Page Intentionally Left Blank
Chapter 1
Constitutive relations for anisotropic materials in linear elasticity 1.1. Introduction Stressstrain or constitutive relations for anisotropic materials will be treated first, and in particular the behaviour of orthotropic and transversely isotropic materials, the latter including unidirectional composites. Then, using tensor notation based on four indices and the conventional notation with two indices, the expressions for changing axes in terms of stresses, strains, stiffnesses and compliances will be detailed.
1.2. Four indices tensor notation 1.2.1. Constitutive relations The reference state is a natural state without stress or strain, that is: trq = 0 and eq = 0 . In linear elasticity theory the stress tensor o is given as a function of the strain tensor E by the tensorial relation: = C e9, or with the indices: o'q = Cqktekl , with i, j , k , I = 1,2,3. The sign
indicates 9 a tensor product. The Cqk I elements are the 81 components
of the elastic moduli tensor or stiffness tensor C. In a homogeneous medium the 81 elastic moduli Cqkt are independent of the point considered. Inversion of the constitutive relation provides the tensor expression: E = S ~9, or using index notation" eq = Soktcrkt . The Sqk I are the 81 components of the elastic compliance in the compliance tensor S.
4
Analysis of composite structures
1.2.2. Properties o f Cijta a n d Sijta
1.2.2.1. Symmetry with respect to the last two indices The stresses are given by: trij = C i j u e u = Cijlkelk . As the strain tensor is symmetrical we have: eta = elk, hence trij = Cijlketa . By identification, the symmetry property is obtained: Cijkl  Cijlk
9
1.2.2.2. Symmetry with respect to the first two indices The stresses are given by: O'ij = Cijkl s , or cr ji = C jikl s
"
As the stress tensor is symmetrical we have: Or(i = O'ji , hence trij = CjitaEkl . By identification, the symmetry property is obtained: Cijkl = C jikl .
1.2.2.3. Symmetry o f the first pair of indices with respect to the second pair From the application of the first law of thermodynamics to elasticity, the state function U, the internal energy, is identified with the strain energy W a . The elementary strain energy per volume: o'ij d E q ,
is an exact derivative: O O'ij _ O 0"ta
Oekl
Oe~j '
with cro = Cijtaeta and trta = Ctaijeij. After introduction in the equality above, we obtain the symmetry property: Cijkl = C k l i j .
Given this property, the elementary volume strain energy: dw d = trqdeij = Cqtaetadeij , leads to, by integration, the volume strain energy:
Constitutive relations for anisotropic materials
5
The compliances have the same symmetry properties as the stiffnesses.
1.3. Conventional two indices Voigt notation
Given the two first symmetry properties: C q k I = C jikl = Cqtk , the order of the first two indices (i, j) and the next two indices (k,l) does not affect the modulus of elasticity values. As there are six distinct values for the group (i, j) and six distinct values for the group (k,/), there remain 36 independent elastic moduli. Given the third symmetry property: Cqkt = Cktq , the permutations of the (i, j) and (k,l) groups do not modify the elastic moduli values. The number of independent values is therefore reduced to 21. Taking account of the previous remarks, we can propose: Cijkl  C Ij , with C tj = C jI , where l=i
for i = j ,
l=9(i+j)
for i;~j,
and J = k for k = l ,
J =9(k+/)for
k;~l.
The index relationship 0./j = Cijktekl being written in the explicit form" 0.ij = Col IE'll + CijE2822 + Cq33833 + 2Cq23E'23 + 2Cq316'31 + 2Cql2E'12 ' the constitutive relation can be written in the matrix form:
"0.11 0"22 0"33 0"23 o'31 O'12
Cllll C1122 Cll22 C2222 Cll33 C2233 C1123 C2223 Cll31 C2231 Clll2 C2212
or in the index form: 0.1 = C I J E J
with the convention:
,
C1133 C2233 C3333 C3323 C3331 C3312
C1123 C2223 C3323 C2323 C2331 C2312
Cll31 C2231 C3331 C2331 C3131 C3112
C1112 C2212 C3312 C2312 C3112 C1212
Ell E22 E33 2c23 2e31 _2e12_
6
Analysis of composite structures
al =crij and l = i
for i = j ,
a l=aij and l = 9  ( i + j )
for i ; e j ,
and:
e s = e u and J = k for k = l , ej=2ekt and J = 9  ( k + l )
for k;el.
The constitutive relation can also be written in the form:
al ! 0"2 0"3 = 04] O'5 _06
J
"Cll Cl2 C13 C14 C15 C16
Cl2 C22 C23 C24 C25 C26
Cl3 C23 C33 C34 C35 C36
Cl4 C24 C34 C44 C45 C46
C15 C25 C35 C45 C55 C56
C16]El. C26 / e2 C36 [ e3 C46 / E4 C56 / E5 C66Ji.s
, or o = C~.
/
/
Similarly we have: El = SIJ oJ, or ~: = So, with S
1.4. Anisotropic
= C 1 .
material
1.4.1. Monoclinic material The monoclinic material studied has the plane (Mlx3,x 1) as a plane of mirror symmetry.
T( ln')
1 n
9
x2
n
M
x2
Figure 1.1. Mirror symmetry axes The two axes in
(e ) XI,X2,X ( ) 3
and
(e')= (x"l,X2,X3 " ") (XI,X2,X 3 )
symmetrical about the plane (M[xa,x I ). The two vectors: n
= nix I +//2x2 + n3x 3 , and
are
Constitutive relations for anisotropic materials n = n i x l  n 2 x 2 +n3x 3 = n i x I +n2x 2 + n 3 x 3 = n i x I +n2x 2 +n3x3, are symmetrical.
The components n i 9of n
in 9
(e') are equal to the
The mirror symmetry property of the two vectors n
*
n i components of n in (e).
and n is written:
n i = rli . ~
t
For the two symmetric stress vectors T(M[n*)and T(MIn ), we have the same: ri* = r i
.
The relation T(M
In)= (o(M))n is written in index form:
T i =O'ijn j in (e),
and:
"" j in = O'ijn
(e') .
Given the preceding remarks, the second relation is written: T/ = o ' q*n j , hence, by identification" o'q = o"0 . The components with the same indices o'/j and crq of stress tensor in the two axes (e ~ and (e)are equal. For the strain tensor we have the same: e(i = eq .
The constitutive relation o = C : c is written in index form: crq = Ciptekl
in the axes (e),
and: * * in the axes (e*) . orij* = CijklEkl
Given the previous properties, the second relation is written: aij = Cqktekt ,
hence, by identification' C•k t = Cok t .
7
8
Analysis of composite structures It
The components with the same indices Cijkl and Cijkl of the stiffness tensor in the two axes (e*)and (e)are equal. Designating by a, the matrix of change of axes from ( e ) t o (e*), the expression for the change of axes for a fourth order tensor is written:
Cok I = a piaqjarkaslCpqrs , and the mirror symmetry property requires: C ijkl = C ijkl . The only nonzero components of the change of axes matrix: a=
are"
~
0
1
0
0
,
all = 1, a22 =  1 , a33 = 1. The elastic modulus CIIII is given by the expression for changing axes" lit
CIIII = aplaqlarlaslCpqrs, where the second index of aij is equal to 1, in the summation for p only all = 1 is not zero, therefore we obtain: C~lll=Cllli
.
The elastic modulus C1112 is, with the same axes change, equal to:
C1112 = aplaqlarlas2Cpqrs, in the summation with as2 only a22 = 1 is not zero, therefore we have:
Clll2 =  C l l l 2
9
The mirror symmetry property Cl112 = CI 112 leads to
Clll2 =  C l l l 2 , hence:
Clll2 = 0 . The elastic moduli which possess the index 2 an odd number of times are zero. The stiffness matrix in the monoclinic axes are thus of the form:
Constitutive relations for anisotropic materials
"Cllll Cl122 C1133 0 C1131 0
Cll22 C2222 C2233 0 C2231 0
9
Cll33 0 Cll31 0 C2233 0 C2231 0 C3333 0 C3331 0 0 C2323 0 C2312 C3331 0 C3131 0 0 C2312 0 C1212
A monoclinic material is characterised by 13 elastic moduli. With the twoindex notation, for the mirror symmetry planer (M[xa,xt), the stiffness matrix is written" Cll
CI2
Cl3
0
Ci5
0
Cl2
C22
C23
0
C25
0
CI3 C23 C33 0 C35 0 0 0 0 C44 0 C46 C~5 C25 C35 0 C55 0 0 0 0 C46 0 C66
1.4.2. Orthotropic material The orthotropic material studied has the two planes (Mlxs,x 1) and (Mix 1, x 2) as planes of mirror symmetry. The nonzero components of the axes that change the matrix from (e) = (x,,x2,x3) to (e*)= (x,,x2,x3)"
a=
I 1 I
0
0
0
1
0
,
0 0 1
are:
all =1, a22 =1, a 3 3 =  1 . According to the previous results, the elastic moduli with the index 3 an odd number of times are zero. The stiffness matrix in the orthotropic axes has the form'
10
Analysisof composite structures
Cllll C1122 C1133 0 0 0 C1122 C2222 C2233 0 0 0 C1133 C2233 C3333 0 0 0 0 0 0 C2323 0 0 0 0 0 0 C3131 0 0 0 0 0 0 C1212, An orthotropic material is characterised by nine elastic moduli. In addition, it is immediately obvious that the (MIx2,x 3) plane is also a plane of mirror symmetry. With the twoindex notation, the stiffness and compliance matrices are respectively equal to:
C
Cil
Cl2
C~3
0
0
0
Cl2
C22
C23
0
0
0
C13 C23 C33
0
0
0
C44
0
0
0
0
0
0
0
0
0
C55
0
0
0
0
0
0
C66
Sl~
Sl2
S~3
0
0
0
Si2 Sl3
$22 $23 $23 $33
0 0
0 0
0 0
and
S ~_
0 0
0 0
0 0
$44 0
0 S5~
0 0
0
0
0
0
0
S66
The inversion of the matrix C involves the calculation of the inverses of the two matrices:
Icc2c31 Ic ~176
II = C12 C22 C23 C13 C23 C33
and b =
0
C55
0
0
0
C66
.
Putting: A = det a = C ! IC22C33 42C12C23C13 we obtain:
 c?
c.
 ci
c...
Constitutive relations for anisotropic materials
Sll=
C22C33  C23
A
C13C23  C12C33
$44 =
'
11
I
C,4 9
'
Sl2=
A
$22 
C l l C 3 3  C~3 A '
S13 =
C12C23  Ct3C22 A '
_ 1 $55  C55'
S33 =
C11C22  C122 A '
S23 
C12Cl3  C23Cll A '
1 S66 = C66 "
The strains are given as a function of the stresses by the matrix relation: El
"Sll
Sl2
Sl3
0
0
0
o"1
E2
$2!
$22
$23
0
0
0
0"2
E3
S31
$32
$33
0
0
0
0"3
E4
0
0
0
$44
0
0
0"4
E5
0
0
0
0
$55
0
o"5
_E6
0
0
O
0
0
The elastic compliances
Sij
$66. .0"6.
can be expressed
as a function
of Y o u n g ' s
moduli E i , the Poisson coefficients vii and the shear moduli G i j . In order to reveal these different values, three simple tensile and three shear tests are proposed. 
In the case of a simple tensile loading in the direction x I , all the or i are zero
except o"I . The strains e i , given by the constitutive relation are equal to: El = S l itYl , e 2 = S2101 , e 3 = S31tYl , e 4 = e 5 = e 6 = 0 . Y o u n g ' s m o d u l u s E l in the x I direction is defined by the relation: E l =J
tY1 J. El x2
x1 i ....................................................................................
Figure 1.2. Simple tension
i
12
Analysis of composite structures The Poisson coefficients VI2 and VI3 are given by:
VI2 E2 = V126.1 =  ~ O ' 1
,
El
and:
V13 6"3 =V136"1 =    O . I
9
El By identification, we obtain: _
1/12
_
VI3.
 In the case of a simple tension loading in the x 2 direction and for a simple tension in the x3 direction, we obtain:
1/21 1 V2~3and 513= v31 v32 1 SI2=~, $22=~, 532 = E2 ~' $23=~3, $33"~.  In the case of a simple shear in the x 2 and x3 directions, all the 0"i are zero except o"4 . X3
a4 I r
J
t
I
0"4
X2
0"4 Figure 1.3. Simple shear The strains e i given by the constitutive relation are equal to:
E4 = $44O. 4 , E l =E 2 =E 3 =E 5 =E 6 =0.
The shear modulus G23 is defined by:
E4 =
O"4 G23
,
Constitutive relations for anisotropic materials
13
hence: 1
$44 = ~ G23  In the case of simple shear in the x3 and x I directions, and in the xl and x2 directions, we obtain" $55 =
l
l
, and $66 = ~ . G31 GI2
 The compliance matrix is written in the orthotropic axes in the form: 1
V21
V31
El vi2
E2 1
E3 v32
El v13
E2 v23
E3 1
El
E2
0
0
0
0
0
0
0
0
0
0
0
E3
0
0
0
0
0
0
0
0
0
0
0
1
G23
1
G31 0
0 1
GI2
and from the symmetry properties of the elastic compliances we have the following relation between the Poisson coefficients and Young's moduli:
vii = vJLi (no summation). E i Ej  The stiffness matrix is obtained by inversion of the compliance matrix and is written, in the axes of orthotropy, in the following form:
Cll
Cl2
Ci3
0
0
0
Ci2
C22
C23
0
0
0
Ci3
C23
C33
0
0
0
0
0
0
C44
0
0
0
0
0
0
C55
0
0
0
0
0
0
C66 _
14
Analysis of composite structures
with: CII = 1  v23V32A El'
C12  v21 +AV23V31 E~,
C13 = v31 +AV32v21 E~,
C21 _ v12 + v13v32 E2 ' A
C22 = 1  v31v13 E2, A C32 _ v23 + v21v13 E3 ' A C55 = G31,
CI 3 _ v32 + v31v12 E2, A C33 = 1v12v21 E3, A C66 = GI2,
C31  v13 + v12v23 E3 ' A C44 = G23, and:
A = 1  2v12v23v31  v12v21  v23v32  v31v13.
1.4.3. T r a n s v e r s e l y i s o t r o p i c m a t e r i a l The transversely isotropic medium proposed here has the (Mlx z,x 3) plane as the isotropic plane. f the (MIx2,x 3) plane is an isotropic plane, the elastic moduli with the same indices in the two axes
~)~ e = xt,x2,x3 )
and
(e)*
=
(x"t , x 2", x 3")
by the following relations: X
I
=Xl,
x 2 = c o s a x 2 + s i n a x 3, X3
=  s i n a x 2 + c o s a x 3,
have the same value whatever the angle ct.
x3 ~ a #
x3 x2
M X1 =
XI
Figure 1.4. Isotropic plane
ho 9 matrix for changing the axes from /e)to (e')
X2
which are defined
Constitutive relations for anisotropic materials
a=
I I
0
0
]
0
cosa
sina
0
sina
cosa d
,
has the following nonzero components: al I = 1, a22 = a33 = COS~, 032 = a23 = sint~. In the particular case where ct = ~, the nonzero components of a are: all = l , a32 = l , a 2 3 =  1 .
Cijkl = apiaqjarkaslCpqrs
The formula for changing the axes Cllll =
aplaqlarlaslCpqrs
C2222 =
ap2aq2ar2as2Cpqrs
= C3333,
C3333 =
ap3aq3ar3as3Cpqrs
= C2222,
= Cllll,
C1122  CI 133,
C2323 " C3232,
C1133 =C1122,
C3131 =C2121,
C2233 = C3322,
C~212  C1313.
The property
Cijkl = Cijk!
provides the relations"
C2222  C3333, Cll22  C1133, C3~3~  C1212" Given these relations, the stiffness matrix: Cllll
C1122 C1122
0
0
0
C1122 C2222 C2233
0
0
0
C1122
0
0
0
0
C2233 C2222 0
0
C2323
0
0
0
0
0
0
C1212
0
0
0
0
0
0
C1212
leads to:
15
16
Analysis of composite structures
involves six independent components. With the twoindex notation we have:
Cll Cl2 Cl2
C12 C22 C23
Cl2 C23 C22
0 0 0
0 0 0
0 0 0
0
0
0
0
0
0
C44
0
0
0
C66
0
0
0
0
0
0
C66 
For any angle 5 we have: a l l =1, a22 = cos 5,
a23 =  sin 5,
a32 = s i n a ,
a33 = c o s 5 .
In the formula for changing axes C2222 =
ap2aq2ar2as2Cpqrs, the
only non
zero ap2 are:
a22 = cos 5 and a32 = sin a , so we obtain"
9
C2222 = cos4 aC2222 + cos 3 5 s i n 5
(c 2223+ C2232 + C2322 + C3222)..
... + cos 2 a, sin 2 5(C2233 + C3322 + C2323 + C2332 + C3223 + C3232)... ... + cosssin 3 5(C2333 + C3332 + C3323 + C3233)+ sin 4 5C3333. With C2222 = C3333, Ciiij = 0 for i r j
(no summation), and introducing the
property Cijkl  Cijkl , we obtain:
C2222 = COS4 5 C2222 + 2 cos 2 5 sin 2 5 (C2233 + 2C2323 )+ sin 4 5 C2222 ,
or (lcos4 5  s i n 4 5)C2222 = 2c0s2 5sin2 a(C2233 + 2C2323), I(cos2 t2' + sin 2 5 ) 2  cos4 5  sin 4 5]C2222 = 2cos 2 5sin 2 5 (C2233 + 2C2323), 2 cos 2 5 sin 2 5 C2222 = 2 cos 2 5 sin 2 5 (C2233 + 2C2323 ). This relation is satisfied whatever the angle 5 if we have: C2222  C2233 + 2C2323
9
The application of the formula for changing axes to other elastic moduli does not result in new relations.
Constitutive relations for anisotropic materials
17
The stiffness matrix is written in the transverse isotropy axes in the following form:
Cllll
C1122
C1122 C2233+ 2C2323 C1122 0 0
C2233 0 0
0
0
C1122
0
0
0
C2233
0
0
0
C2233 + 2C2323 0 0 0 C2323 0 0 0 C1212 0
0
0
0 0 0 C1212
A transversely isotropic medium is characterised by five independent elastic moduli. Certain unidirectional fibre composites can be considered as transversely isotropic materials. With the twoindex notation we have'
Cll Cl2 Cl2 0 0 0
Ci2 C23 +2C44 C23 0 0 0
Cl2 C23 C23 + 2C44 0 0 0
0 0 0 C44 0 0
0 0 0 0 C66 0
0 0 0 0 0 C66.
1.4.4. lsotropic material In an isotropic material all directions are equivalent. In axes (e)=(Xl,X2,X3)and
(e') = ( x l , x 3 , x , ) t h e
Cijkl and
Cijkl
components
with the same indices have the same numerical value. The only nonzero terms of the change in axes matrix:
I
0 0 11 1 0 0,
a=
0
are:
1 0
a21 =1, a32 =1, a13 =1. The formula for changing axes: llt
Cijkl = a p i a q j a r k a s l C p q r s
with the property: C ijkl  C ijkl '
providing the relations:
,
18
Analysis of composite structures C l l l l = C2222,
C1122 = C2233,
C2323 = C3131,
C2222 = C3333,
C1133 = C2211,
C313] =C1212,
C3333 = C l l l l ,
C2233 =C3311,
C1212 = C2323,
or:
CIIII = C2222 = C333, C1122 = C2233 = C3311, C2323  C3131  C1212.
Putting C2233 = ,~ and C2323 = ,t/, the relation C2222 = C2233 + 2C2323 gives: C2222 = ,~, + 2,//. In all axes, the stiffness matrix is written in the following form:
A,+2/l A, 2, 0 0 0
A, 2+2,u A, 0 0 0
A, 2, 2,+2,u 0 0 0
0 0 0" 0 0 0 0 0 0 ,u 0 0 0 ,u 0 0 0 /z
An isotropic material is characterised by the two elastic moduli ,,l and /z termed the Lam6 coefficient, or by Young's modulus E and by Poisson's coefficient v. We recall the relations: vE E ,,l=(l+vXl_2v), ,u=G=2(l+v) E /L(32 + 2,U) ,'1, it+,/, ' 2(2 +p)" Determination of the compliance matrix involves the following expressions A = ( 2 + 2/L)3 + 2 3 3  3 2 ( 2 + 2/~) = 4/t2 (3a + 2~t), + 2**)2 _ a2
all 
4/z2 (32 + 2/z)
S, 2 = _ 2 ( A + 2/t) A2 4,u2 (3,;t + 2,u) 1 l+v $44 =   = 2 ~ . ,u E
2+~
1
/z(32 + 2/t)
E
,~,
V
2,u(3,;t + 2/z)
E
Constitutive relations for anisotropic materials
19
The compliance matrix is written in all axes as' 1
v
v
E v
E 1
E v
E E v v . . . . . E E 0
0
E 1 E
0
0
0
0
0
0
0
0
0
0
0
0
0
2 l+eE
0
0
0
l+v 2E
0
0
0
0
0
2 .+__.:_. E
1.4.5. Influence o f temperature a n d humidity on the constitutive relation o f an orthotropic material The variation of temperature AT results in a strain field defined by' e, = oti A T (i = 1,2,3), e i = 0 (i = 4,5,6), or:
ei=ctiAT
( i = l , 2 ..... 6), with ct4 = c t 5 = c t 6 = 0 .
oti being the coefficient of thermal expansion in the x I direction.
The variation of humidity At/, equal to the relative variation of the mass of the material, results in a strain field defined by: e, = fliArl (i : 1,2,3), e i = 0 (i : 4,5,6), or:
e, = fliArl (i = 1,2 ..... 6), with ,84 = r5 = ,86 = 0. ,8i being the coefficient of hygroscopic expansion in the x I direction.
In general the elastic moduli depend on the temperature and the humidity. When the temperature and humidity variations are small, the elastic moduli can be assumed to be constant. Taking into account the strains caused by the stress field due to the variations in temperature and humidity, the constitutive relation is written as: e i = S o t r j + otiAT + fliArl (i, j = 1,2,3), e i = Sqtrj or:
(i, j = 4,5,6),
20
Analysis of composite structures ~ei = Sijo" j + Gt,i A T + i~iAl~ (i, j = 1,2 ..... 6),
a,i =0, ,Bi = 0 (i =4,5,6). In the orthotropic axes the thermal and hygroscopic effects are revealed as expansions in the x I direction, and by the absence of angular distortion in the x i and xj directions.
1.5. Matrix relations for a change of axes
In the direct orthotropic axes (~)= ( X i , X 2,X3), the constitutive relations are written: =C[ andg=Sfi. Whereas in the offaxis coordinates (e)= ( x i , x 2 , x 3), we have" o = C E and c = S o . The matrix for changing axes from (~) to (e)is represented by a:
a =
~
a 21
a22
a23
a31
a32
a33
9
1.5.1. Change of axes for stress and strain matrices The following formula is proposed for the change of axes matrix: O'ij = a pi a qj O'pq
in matrix form: o = M~ , where M is a (6,6) matrix which will be determined. The explicit expressions: O'11 = a p l a q l O ' p q ,
O'll = a121~'l i + alla21ffl2 + alla31ffl3... ... + a21a I iOr'21+a21~22 + a21a31ff23... ... + a31al IO'"31+ a31a21cr'32 + a21~33, and: m
0"23 = ap2aq30rpq ,
Constitutive relations for anisotropic materials m
. . . .
21
m
0"23 = a12a130"11 + a12a23012 + a12a33013"" ... + a 2 2 a 1 3 0 " 2 1 + a 2 2 a 2 3 0  2 2
+ a22a33023...
... + a32a13031 + a32023032 + a32a330"33,
enable the change of axes formula to be written in the matrix form: 0"11
al21
a22,
a3t2
2a 21a3 l
0"22
a122
a222
a~2
2a22a32
0"33
a23
a223
a~3
2a23a33
023
a12a13
a22a23
a32a33
a22a33+a32a23
0"31
al3al I
a23a21
a33a31
a23a31 + a33a21
_0"12 _
al la12
a21a22
a31a32
a21a32 + a31a22
, , .
2a31all 2a32at2 2a33at3
2alla2t 2a12a22 2al3a23
a32a13+a12a33
a12aE3+a22a13
a33atl + a13aat
a13a21+a23att
a31ai2 +alia32
alla22 + aElal2
_O'12 J
The matrix M is made up of four submatrices (3,3) whose components can easily be found by writing the transposed change of axes matrix: 8r
=
i!l a ~ 12
a22
a32
13
023
~
9
Decomposing the matrix M in four submatrices (3,3): M =
tt
Mr2
2t
M22
,
the following rules can be proposed:  The (i, j) component of the submatrix i , ,
is equal to the square of the (i, j)
component of a t .  The (i, j) component of the submatrix Mr2 is equal to twice the product of the two other terms of the row i of a r .  The (i, j) component of the submatrix M21 is equal to the product of the two other terms of the column j of a t .
22
Analysis of composite structures  The (i, j) component of the submatrix M22 is equal to the sum of the cross
products of the terms of the matrix obtained by removing row i and column j of a t . In a similar manner we can develop the formula for changing the axes of the strains" Eij = a p i a q j E p q ,
in matrix form: = N~, with N being a (6,6) matrix which will be determined. The explicit expressions: m
~'11 =aplaqlCpq, ell = a?l~'l i + alla21e'12 + alla31e13... 
2
... + a 2 1 a l l E 2 1 + a 2 1 E 2 2 + a21a31E'23...
... + a31al 1~'31 + a31a21~'32 + a321~33,
and: E23 = d p 2 a q 3 E p q , E23 = aI2aI3EII + a12d23EI2 + aI2a33EI3"" ... + a22a13E21+a22a23C22 + a22a33E23...
... 4 a32dI3E31 + a32a23s
+ a32d33E33,
enable the formula for changing axes to be put in the form" Ell
a?:
E22 s
2e23 2e3~ ]
.2r
aeea3:
=
2al2al3
2a22a23 2a32a33 a22a33+a32a23
2al3al I
2a23all
2a33a31
a23a31 + a33a21
2a I lal2
2a21d22
2a31a32
a21032 t a31a22 m
a31all
alia21
a 32 a 12
a 12 a 22
a 33 a 13
a 13 a 23
a32a13 + a 1 2 a 3 3
a12a23 + a 2 2 d 1 3
a33all +a13a31
a13a21 + a 2 3 a l l
a31a12 + a l i a 3 2
alia22 +a21al2
fll s E33 2e23 2e31 _2et2
Constitutive relations for anisotropic materials
23
N,J
As for the matrix M, the matrix:
9
21 Nz2
consists of four submatrices (3,3) whose components are found as follows"  The component
(i, j)
of the submatrix Nil is equal to the square of the
component (i, j) of a t .  The component (i, j) of the submatrix Nl2 is equal to the product of the two other terms of the row i of a t .  The component (i, j) of the submatrix N21 is equal to twice the product of the two other terms of the column j of a t .  The component (i, j) of the submatrix N22 is equal to the sum of the cross products of the terms of the matrix obtained by removing row i and column j of a t . From the matrix a, we construct the matrix M such that o = Md. Similarly from a l , we can construct, in an analogous manner, the matrix M l such that: ~= MIo. The matrix a  t = a r
is obtained by exchanging the indices i and j of the
orthogonal matrix a. The matrix M l is obtained by exchanging the indices i and j of the terms aij which are involved in the matrix M, which results in: _
a121
al22
al23
2d12013
2al3al i 2dlla12 2a23a21 2a21a22 M 1 = a21 a22 a323 2d32033 2033a31 2a31d32 021a31 d22a32 023033 d22033+d23r a23d31 +a21d33 a21d32+a22d31 a33all "t'a31r a31d12+a32dll r a32r a33a13 a32a13+r _tllla21 a12a22 013023 a12d23+tl13a22 d13d21 +dllt/23 dlld22 +a12a21. The matrix thus obtained is the transposed matrix N. We therefore have the relation: M l = N r ' An analogous calculation, performed on the N matrix gives the equation: N l = M r"
24
Analysis of composite structures
1.5.2. Change of axes for stiffness and compliance matrices We have just obtained the following relations:
=M~
[1], ~ = N r a
c=N'~
[3],
[2],
~=Mrc
[4].
In addition, the constitutive relations in the othotropic axes and offaxis are written"
=CE
[5], [ = S ~
[7],
[6],
[8].
ty=Cr
c=Sty
From relations [1 ], [5] and [4], we obtain: tv = M ~ = M C ~ = M C M r c . Identification with [6] gives: C = MCM r . From relations [3], [7] and [2], we obtain in a similar way: = N~ = NS~ = NSNTtv. Identification with [8] leads to: S = NSN r . Multiplication of the left hand part of C = M C M r by N gives: NrCN = NrM~MrN,
by N r and the right hand part
or"
= NrCN. Multiplication of the members of S = NSN r by M r on the left and by M on the fight gives the equation: MrSM = MrNSNrM, hence: S=MrSM.
Chapter 2
Orthotropic layer behaviour 2.1. Introduction The expressions developed in the previous chapter for the change of axes will now be applied to an orthotropic ply of any orientation in a composite. In the plate theories which will be presented the assumption is made that the normal stress in the x3 direction is zero. This hypothesis leads to the introduction of column matrices of stresses and strains with only five terms. From these we will deduce the formulae for changing coordinates and the constitutive relations which will be used in the plate theories.
2.2. Stiffness and compliance matrices In orthotropic coordinates The orthoptropic layer studied here has the coordinate axes (OlX 1, X2,x 3). The layer of thickness h is limited by the two planes perpendicular to (Olx3) which are defined by x 3 = ~ and x 3 =  h 2'
X2
iiiii!iiiiiii!i!!!iiiii iiiiiill V
XI
Figure 2.1. Orthotropic axes In the following, all the quantities defined in the orthotropic axes will be overscored.
26
Analysisof composite structures In the orthotropic axes (F)= (Xl,X2,x3) the constitutive relation is expressed
as: R
~=S:~, and in the matrix form as: S~, or: =
El
SII
Sl2
Sl3
0
0
0
'~l
E2
S12
$22
$23
0
0
0
0"2
u
E3
o"3
S13 0
$23 O
$33 0
O S~
O 0
O O
O"4
E5
m
0
0
0
0
$55
0
O"5
m
0
O
0
O
O
E4 .~6 _
D
$66  .0"6 _
The compliance matrix can be written in terms of Young's moduli Poisson coefficients
S=
vii and the shear moduli Gij
1
V21
1/31
El vl2 El VI3 El
E2 1
E3 V32
E2
E3
1 E3
V23 E2
in the form:
0
0
0
0
0
0
0
0
0
0
0
1
0
O
0
0
0
0
0
0
0
0
0
G23
9
1
G31 1
0
Gl2
with:
vO= vjji (no summation). e, ej If the plane (X 2, x 3) is a plane of isotropy, then: w
~
m
I
m
u
S22 S33 S23 +7 S.~, S~3 Sl2, S~ =
=
=
L
m
=
s55,
or"
1
E2
1 l = ~ = ~
E3
V32 ~, V21 =V31,
2G23 E3
1
GI2
=
1
G31
Ei,
the
Orthotropic layer behaviour
27
A unidirectional layer in which the fibres are parallel to X t can, for a first approximation, be considered as transversely isotropic. The relation E = S ~ is then written as" 
m
E!


m
m
S12
Sll
S12
E2
"

O.I n
0
0
0
o
o
o
O"2
$23
$23 + r S%
0
0
0
O"3
E4
S12 0
0
0
$44
0
0
O"4
E5
0
0
0
0
$66
0
O"5
.E6.
0
0
0
0
0
m
E3

$66_ .O'6 _
Similarly in the orthotropic axes (~) the constitutive relation: 
...
8"=C:c, can be written in matrix form as: ~=CE, or: 
u
o.l
m

o"2 m
o"3 O"4
o"5 m
_~ _
m
Cl2
Cl3
. . .
.,.
C12
C22
C23
C13
C23
C33
0 0 0
0
0
C44
CII
0 0 _0
0 0 0
0 0 0
0
0 0
..,.
0
0
0
C55
0
0
0
0
C66 e 6 J
In the particular case of the transversely isotropic unidirectional layer we then have: 

_
Cll
B
. . 
Ct2
Ct2
0
0
0
El
0"2
CI2
C23 + 2C44
C23
0
0
0
E2
0"3
Cl2
C23
0"4
0
0
C23 + 2C44 0
0 C44
0 0
0 0
E4
0"5
0
0
0
0
C~
0
E5
_0"6_
0
0
0
0
0

m
o.l


n

E3
C66 .E6.
2.3. Conventional matrices for changing axes The angle a between the vector x I of the offaxes (e) = (x 1, x 2, x 3) and the vector X! of the orthotropic axes (~)= ( X I , X I , x 3 ) , is measured on x 3.
28
Analysis of composite structures
Figure 2.2. Offaxis directions The matrix which enables us to go from the orthotropic directions (~') to the offaxis directions (e)"
a
=
I Ic s!l 
cosa sina sin cr coscx
!1
,
0
o
is written in the form:
II =
$
C
0
0
,
with: c = cos a and s = sin a . From the transposed matrix of the axis change
Ill T
=
Iis !1 C
,
0
we obtain the following two matrices M and N:
i
"r 2
s2
0
0
0
2cs
$2
c2
0
0
0
c$
0
0
0
0
1
0
0
0
s
0
0
0
0
c
$
0
c
0
0
0
0
s
c
0
0
2 _$2
c2
s2
0
0
0
 2cs
s2
c2
0
0
0
0
0
1
0
0
0
0
c
0
0
Os
cs
cs
0
0
0
c2s
,N=
2cs
 2cs
0
0
 
c
c$
Orthotropic layer behaviour
29
2.4. Stress and strain matrices The f o r m u l a e for c h a n g i n g the directions for o = M ~
and ~ = N T o
can be
written in the f o l l o w i n g f o r m s '
cr, ] cr2[ 0"3[ Crn] as] I
c2
s2
0
0
0
 2cs
0.1
s2
c2
0
0
0
2cs
0.2
0
0
1
0
0
0
0.3
0
0
0
c
s
0
o"4
I
.~
u
.J
9
0
0
0
s
c
0
0.5
cs
 cs
0
0
0
c 2 s 2
.0"6 _
and: "
2
2
0
0
0
2cs
'0.1
cX
0
0
0
 2cs
o" 2
0
0
1
0
0
0
o"3
0"4
0
0
0
c
s
0
0"4
0"5
0
0
0
s
c
0
0"5
cs
0
0
0
c2s
0.1
c
0"2
s
o' 3
_~ _
2

cs
s
2 _0"6 _
similarly, the f o r m u l a e for c h a n g i n g the strain axes for strains c = N~ and ~ = M r can be written: 
i
c2
s2
0
0
0
cs
ci
62
s2
c2
0
0
0
cs
E2
63
0
0
1
0
0
0
c3
E4
0
0
0
c
s
0
C4
E"5
0
0
0
s
c
0
_g6 _
_2cs
2cs
0
0
0
c2s

m
C5 2 _E6 _
and: 
El
c
2
s2
0
0
0
cs
El
F.2
s2
c2
0
0
0
cs
E2
~3
0
0
1
0
0
0
E3
C4
0
0
0
c
s
0
E4
0
e5
m

F.5
0
0
0
s
c
.C6.
 2cs
2cs
0
0
0
c 2  s 2 _E6.
9
30
Analysisof composite structures
In the present case it may be noted that we go from M to its inverse N r by replacing the angle a by  a in M. One can use the same transformation to go from N to its inverse M r . 2.5. Stiffness matrix in directions away from the orthotroptc axes
The stiffness matrix C in the (e) space is given by the relationship: C = MCM T
I
which involves the matrix:
m
c2
s2
0
0
0
 2cs
s2
c2
0
0
0
2cs
0
0
1
0
0
0
0
0
0
c
0
0
Os
cs
cs
__
0
0
s
0
c
0
0
c2s
2
The product of the latter two matrices is thus: l
~Mr=]C,3 i
Cl2
"Cl3
0
0
0
c2
o
o
o
$2
0 0
0 0
i
C'23 C33 0 0 0 C,.4 0
0
0
Css
o
o
o
o
0
0
0
o
o
o
.
0 0
1 0 0 0 c s
i
0
0
s2
0
c~JL2c~
2~
s
c
o o
o
cs
' c ~~j
that is:
~M r
c2C'11 + $2C'12 $2 C'll + C2~'12 CI 3
0
0
c~e,~ +~c~ ~'e,~+c~e~ c~ c~c,3+~c%3 ,'Cl~+c~e~3 c%3
o o
o o sC~
0
0
0
cC~
0
0
0
sCss
cCss
 2csC66
2csC66
0
0
0
.(~,,c,,)c,(e,, c~,) c,(~,, c%) 0 0 (c 2  s2)~'66.
After multiplying the lefthand side by M and identification, one obtains:
Orthotropic layer behaviour 
the components of the first column of
C:
Cl, : c4C'11 + s'lC'22 + 2c2s2 (C'12 + 2C'66 ),
C2, :cZs2('C,, +C"224~'66)+(c 4 + s')C,2, C31 = c2C53 + 12823 , C41 = O , C51 =0, C6 ' =r162 _$2~'22 _(r 
_$2)(~"2 +2C" )l,
the components of the second column of C: C,2 = c2s2(Cl, +C'224C'66)+ (c4 + s4)C~2 =C2,,
c,2 ~'e,, +~'c5, + 2c~(e,, + 2e~), C32 = 82C'13 + c2C53 , C42 = 0, C52 = O,

the components of the third column of C:
C13 = c2C"13 + 82823 = C31, C23 = $2C"13 + r
= C32,
C33 = C33, C43 = O, C53 = O,
c~3  c~(e,, c%), 
the components of the fourth column of C: Cl4 = O, C24 = O, C34 = O, C44 = c2C'44 + s2C'55,
c,, = ~,(e,, ~,,), C64 = O,
31
32
A n a l y s i s o f c o m p o s i t e structures
 the components of the fifth column of C: Cl5 = O,
C25 = 0 ,
C35 = O, c., =
c,..
C65 =0,  the components of the sixth column of C:
2 + 2C66

2 +
= C61,
2C66
=
C62,
C36 = cs(C'13 C23)= C63, C46 = 0, C56 = 0,
The constitutive relation o = Ce can then be written as:
oI o"2 o"3
C l 6 "El C26 s C36 E3 .
C12 C22 C23
Cl3 C23 C33
0 0 0
0 0 0
o 4
Cll C12 C13 0
0
0
C44
C45
0
E4
o5
0
0
0
C45
C55
0
C5
_o6
C16
C26
C36
0
0
C66 _E6
Note that for a = 0 or a = {, the coefficients C16, C26 , C36 and C45 are equal to zero ( orthotropic materials whose directions of orthotropy coincide with the coordinate axes). 2.6. Compliance matrix in directions away from the orthotropic axes The compliance matrix S in (e) is given by the relationship:
S = NSN T which involves the matrix:
Orthotropic layer behaviour 2
0
0
0
cs
S2
C2
0
0
0
cs
0
0
1
0
0
0
0
0
0
c
0
0
Os
2cs
 2cs
r
N
,..
2
S
0
0
s
0
c
0
0
c2s
The product of these two matrices is: m
Sll Sl2 SI3 0
gN r
s,~ s,~ s~, s53
o o
o o
o o
c2 s2
s2
0
0
0
2cs
c2
0
0
0
 2cs
sS~ sL~
o
o
o
0
0
1
0
0
0
0
0
c
s
0
0
0
0
$44
0
0
0
0
0
0
S55
0
0
0
0
s
c
0
cs
cs
0
0
0
c2  s2
0
0
0
0
0
$66
 
that is'
~.. +~.~ c2S~2 + s2922 ~.~+c~s~
~.~ ~.
o o
o o
2.(~..~.~) 2.(~.~s~)
0
0
cS44
" sS44
0
0
0
sS55
cS55
0
0
0
0
(C2__ S 2 )~'66
c 2s~3 + s 2g23
gN r
0
0
r
 csS66
After multiplication of the lefthand side by N and identification, one obtains:  the components of the first column of S"
Sit
t
s~.
=C2 s 2( ~ . . + ~
2
_
~)+
(r
+ S4)~12 '
 + S 2 $23, $31 = C2 S13 S4t = 0, SsI = O, $61 = c s [ 2 c 2 S 1 1  2 5 2 S ' 2 2  (
C2 " s2)(2S'12 + S'66)],
33
34
Analysis of composite structures  the components of the second column of S:
SI2 = r S22 =
+ 8 2 2  S'66)+ (C4 + s4)8"12 =$21 ,
$4Sli + c4S'22 +r
+ S'66~
$32 = $2,~'13 + c2S'23 , $42 =0,
$52 =O,
S62 =c$[2525'I" 2c2S'22 +( c2 $2)(2512 + 566)],  the components of the third column of S:
S13 = c25"13 +
$2523 = 831 ,
$23 = $25"13 + c25"23 = $32 , $33 = $33 , $43 =0,
$53 =O, $63 = 2r (513  $23 ),  the components of the fourth column of S:
514 =0, $24 = O, $34  O, s.
=r
+ ~'g.,
S54 = c ' ( 5 5 5  g 4 4 ~
$64 = 0 ,  the components of the fifth column of S: $15 = O, $25 = O,
$35 =0, s55 = s 2 944 + c2S55, $65 = 0 ,
Orthotropic layer behaviour
35
 the components of the sixth column of S:
$36" 2c5(S'13  S'23) = S63 , $46 = 0 , $56 =0, $66 = 4c2s2(S'~1 +S'22 2S'~2)+ (c2 s2)2S~
9
The constitutive relation ~ = S~ can then be written as' SII
S12
S13
0
0
S16
0.1
S12
$22
$23
0
0
$26
o"2
E3 = S13 0 E4
$23 0
$33 0
0 S44
0 S45
$36 0
0"3 .
0
0
$45
$55
0
$36
0
0
ie5 i ~.E6.
0
_S16 $26
0"4
~ $ 6 6 _0.6 J
As for the stiffnesses, note that for the compliances SI6, $26, $36 and $45 are
zero for a = 0 or ct = ff (orthotropic axes coincide with the coordinate axes).
2.7. Orthotropic layer loaded in tension and in she[r 2.7.1. Simple tension For the case of a layer loaded in simple tension in the xl direction, the only nonzero component of the matrix is 0.1.
Xl
Xl 0.1 Figure 2.3. Tension offaxis
36
Analysis of composite structures The constitutive relation c = So gives" E l = SllO'l , E 2  S120"1, E3  S130rl,
s
=0,
~75 = 0 , E6  S160"1. The layer undergoes three unit extensions in the x I , x z and x 3 directions as well as an angular distortion in the two orthogonal directions xl and x z. For a = 0 (fibres parallel to x I ) or ct = ~ (fibres parallel to x 2), the elastic compliance S l6 is zero. The angular distortion is then zero. The strains obtained are shown in the figures below.
kx2
Figure 2.4. Strains when St6 g 0
Ak x2
v
O
Figure 2.5. Strains when Sl6 = 0
x
Orthotropic layer behaviour
37
2.7.2. Simple shear W h e n the layer described previously is loaded in simple shear in the two directions x I and x 2, the only c o m p o n e n t which is not zero in the stress matrix is 0"6.
a6
0" 6 Figure 2.6. Shear in offaxis directions
Given the constitutive relation ~: = S o , we have" E I = Sl60.6.
E4 = 0,
E2 = $260"6 ,
E5 = 0,
E3 = $360. 6,
E6 = $660. 6.
The layer undergoes unit extensions in the x I , x 2 and x a directions, and an angular distortion in the two directions xt and x2. For ct = 0
or a = g, 2 the elastic compliances S i 6 , $26 and $36 are zero. The
linear expansions are therefore zero. The corresponding strains are represented by the following figures.
O
Xl
Figure 2.7. Strains when Sl6 r 0, $26 ~ 0,$36 ~ 0
38
Analysis of composite structures
A~ x2
xI
Figure 2.8. Strains when S!6 = $26  536  0
2.8. Reduced stiffness matrix for the orthotropic layer In this paragraph, we will describe the Q and Q of an orthotropic layer with through thickness normal stress tr 3 zero. These matrices are introduced into the theorems of KirchhoffLove and ReissnerMindlin for multilayer materials.
2.8.1. Reduced stiffness matrix Q in orthotropic coordinates In the orthotropic coordinates (E), the constitutive relation ~ = C ~ is written as: o"1
Cll
Cl2
Cl3
I
_
!
0
0
0
o"2
C12
C22
Cl
C23
0
0
0
E2
o"3
C13
C23
C33
0
0
0
c3
o"4 o"5
0
0
0
C44
0
0
E4
0
0
0
0
C55
0
C5
_~ _
0
0
0
0
0
C66
_C6 _
_
1 0
Whena 3  CI3~ ! + C23~2 + C33E3 = 0 , the expansion ~3 is equal to:
C~3~ + c23~2
E3 =
__ (?33 The normal stresses"
.
a~ = C~ t~ + C~2~2 + c~3~3, 

1
i
a2 = C~2~ + C22~2 + C23~3,
Orthotropic layer behaviour
39
can then be expressed only in terms of El and e2, using:
~1 = ell'~'~331 ~1 + C 1 2 
C"3"~
C33
E2,
El + e22  C"3"~'3" ~'2 '
By putting: Cix
_
QII = CII
_
_
C'33'
QI2 = c12 
_
Q22 = C22
C'73 C'33'
Q~66 = C66'
C13C23
C33
Q44 = C44, Q55 = C55, the constitutive relation can be expressed in one of the following two forms:
~, r~,, ~,~ e4 .~ or:
o
o o
o~,
o
o
o ;g4 ~5 : ~
~o,,:1
II
o][;,7
with: __
_
a,j = %
Q~j = C~j
Ci3Cj3
~(i,
j = 1,2),
c.
(i, j = 4,5,6).
In the plate theorems of KirchhoffLove and ReissnerMindlin we keep the notations ~ and ~ to represent the matrix columns of stress components' O"1,O"2,O"6,O'4,O"5 , or O"1,0.2,0. 6 ,
and strains" EI,E2,E6,E4,E5, or s which have just been introduced, and designate by Q the corresponding reduced stiffness matrix.
40
Analysis of composite structures
2.8.2. R e d u c e d s t i f f n e s s m a t r i x Q in t h e c o  o r d i n a t e s a w a y f r o m t h e o r t h o t r o p i c axes
The change from the orthotropic axes (~) to the offaxis coordinates (e) and its transposition are written as:
a =
c
and a r =
c
0
.
0
The matrix axes change with respect to the stresses tt = M6, involving the matrix: C S M
_.
2
$
2
C
2
0
0
0
 2cs
2
0
0
0
2cs
0
0
1
0
0
0
0
0
0
c
s
0
0
0
0
s
c
0
C$
 C$
0
0
0
c2  s2
can be written for this case in the form"  2cs
0
0
c2
2cs
0
0
cs
cs
c 2 s 2
0
0
0"4
0
0
0
c
s
0"5
0
0
0
s
c
0.1
c2
0" 2
s2
0"6
=
s2
io,l c2 s2 _2csI"l
or:
0.2
= s2
0" 6
C$
c2
2cs
~2
C$
C2$ 2
5 6
[o,][:,
],
keeping the notation M for the two new conventional change of axes matrices associated with the two matrices of the stress components 51, 52 , 56 , 54 , 55 and ~
~
0.1,0.2,O'6
.
r = l~r
The formula for changing the axes with respect to the strain matrices E = N ~ , with:
Orthotropic layer behaviour
c2
s2
0
0
0
cs
$2
c2
0
0
0
cs
0
0
1
0
0
0
0
0
0
c
0
0
Os
2cs
 2cs
S
0
0
s
0
c
0
0
c2  s2
41
can be written as:
or:
e l
c2
s2
 cs
0
0
"el
e2
s2
c2
cs
0
0
e2
e~  o2C~  2~ ~  ~
o
o~ ~ ,
e4
0
0
C
E4
:5.
0
0
 s
.e5
,li
E2
e6
c2 s2 _cs
=
S2
C2
CS
2cs
 2cs
c 2 _ S2
E'2
,
E:,'IE:,
cjLg5 ]"
So, by designating as N the new conventional axis change matrix" ~=N~. The formula for changing C = MCMr Q
axes, established
for the
stiffness
matrices
leads to the relation:
= MQM r .
Given the calculations already performed for the change of axes the reduced stiffness matrix Q is of the form:
Q ._
with:
QII
QI2
QI6
0
0
QI2
Q22
Q26
0
0
QI6
Q26
Q66
0
0
0
0
0
Q44
Q45
0
0
0
Q45
Q55_
42
Analysis of composite structures
QII =C4QII +$4Q22 +2c252(~2 +2Q66) ,
Q,2 = c2s2(~, + Q224Q'66)+(c4 + s4)~2, QI6 = C$[c2Q11 $2Q'22 "(C2 $2)(~2 + 2Q'66)1,
Q~0 c,[,~, c~2 + (c~,~)(o,~ + ~)1, 2
Q44 = c2044 + s Qss,
Q45 = C$(J~5 Q'44)" It should be noted that the reduced stiffnesses Ql6, Q26 and Q45 are zero for ct = 0 or a' = ~. These relationships can be written in matrix form" 
.
C4 $4 C2S 2 C2S2
QII Q22 Ql2
Q6~ Ql6 = Q26
S4 C4 C2S2 C252
2C2S 2 2C2$2 C4 +$4
4C2S 2 4C2$ 2 4C2S 2
0 0 0
0 0 0
 2C252
(c2 7" S2)z
0
0
c~,  c , ~  c , ( c ~  , ~ )  ~ , ( c ~  , ~ )
o
o
Q44
0
0
0
0
c2
s2
Q55
0
0
0
0
s2
c2
_Q45
0
0
0
0
C4
S4
S4 C252 C2S2
C4 C252 C2$ 2
2c2s 2 2C2S2 C4 + S4 2C2S 2
4c2s 2 4C2S 2 __4C2S2 ~ 2 $ 2 ~
cs
or:
QIi ]
Ql61
_e,~~, c,i~,~) ~c~i~,~).
_Q26J
Q44 Qs5
/Q~5
]
=
c2 S2 c~
$2
CS Q55
Q~
cs
_0"55
Orthotropic layer behaviour
43
2.9. Reduced compliance matrices of an orthotroplc layer Having presented the reduced stiffness matrix Q
we will now derive the
reduced compliance matrices P and P for an orthotropic layer where the throughthickness normal stress o"3 is zero.
2.9.1. Reduced compliance matrix in orthotropic coordinates In the orthotropic coordinates we have" 
m
Pl2
0
0
0
"~'l"
~2
~2
o
o
o
~2
E6 =
0
0
P66
0
0
~6 ,
~'4
0
o o
o o
~e2 m
m
0
_E5
~44 o ~4 o ~55 ~5
with: m
Pll
=
m
Q22 , QllQ22 _ ~  2
~22=
QII
1

P44 = g44'
1 2 = _ P
QI2 , QI iQ22  Ol~
~66=
1

l
P55  55"
2.9.2. Reduced compliance matrix P in the direction away from the orthotropic axes The formula for the change in coordinates for the reduced compliance matrix is written as" P = N~N r Given the preceding calculations for changing axes the reduced compliance matrix P may be written as'
ell p
.
e12
el6
Pl2 P22 P26 Pl6 P26 P66 0
0
0
0
0
0
0
0
0
0
0
0
P44 P45 P45 P55
,
44
Analysis of composite structures
with:
el2 =c2$2('P111+P22P66)+ (c4 + s')ell2, P66 = 4 c 2 s 2 ( ~ , +  f i n  2 ~ 2 ) + ( c 2  s 2 ~ f 6 6 , PI6 =c$[2c2pII1 2$2P22( c2 $2)(2P112 + P'66)1.
P55 = s2p44 + c2~5, It may be noted that the terms el6. P26 and P45 are zero for ct = 0 or ct = n_. 2" These relationships can be presented in the form: C4
Pll
s4
2C2S 2
c2s 2
0
0
~2
S4
C4
2C2S 2
C2S 2
0
0
~2 P66
C 2s2
C2S 2
C4 +S 4
C2S 2
0
0
 8 c, 2 s 2
(c 2 ,  s 2 ~
i
4c2s24c2s
2
O 0
 2cs 3
~6 P44 P55
0
0
0
0
c2
s2
0
0
0
0
S2
c2
.P45 _
0
0
0
0
 cs
CS
C4
s4
2c2s 2
c2s 2
S4
4
2c2s 2
c2s 2
C2S 2
c c2s 2
c 4 + s4
_c2s2
P66
4C 2 S 2
4c 2 s 2
8c2s 2
(c 2  s 2 ~
P~6
2C3S
 2CS 3
_P26 _
2CS 3
2C3S
 2cs[c 2  s 2
P66
(.
or" ell

P22 PI2
P44
C2
P55 =
s2
LP45
 cs
S2 CS
"P55 "
2c,(c_,i)
I Pl2
2c3s
!PI6 =
P22
P_22,
52
P66
_ sJ
Chapter 3
Elastic constants of a unidirectional composite 3.1. Introduction When an orthotropic material is in a plane stress state the relationships between the stresses and strains involve the four elastic constants E l , E 2 , I,'12 and GI2. In addition to these coefficients, when considering thermoelasticity the coefficients of thermal expansion cq and or2 are also required. In this chapter we are able to obtain the characteristics of a unidirectional composite material as a function of the characteristics of the fibres and the matrix.
3.2. Density p Designating as:  M,
M r , M m the masses of the composite, fibres and matrix,
 p, ,of, /9m the densities of the composite, fibres and matrix,  v, v f , v m the volumes of the composite, fibres and matrix,
the mass of the composite is" M =Mf
+M m ,
or:
pV m p f V f
+PmVm
9
Then: Vf =
vf
v
, the volume fraction of the fibres,
V m = vm
v
the volume fraction of the matrix,
and noting that V f + V m  1, the density of the composite is: p = V/ p / + VmP m = V / p [
+ (l  V f )p m .
46
Analysis of composite structures
3.3. Longitudinal Young's modulus E l In the theory below we assume that, as shown in the figure, the fibres are concentrated in the lower part of the composite and that the matrix occupies the upper part. The composite is subjected to the longitudinal tensile force F.
~
X2
I V
FX l
matrix
X1
fibres Figure 3.1. Longitudinal tension In the model adopted here, we suppose that the longitudinal extensions resulting from the tensile force F are the same in the composite, fibres and matrix, which can be presented as: e I = e lf = e ~ .
We designate as:  E l, , E m the Young's moduli of the fibres and matrix, S m the surface areas, orthogonal to X l , occupied by the composite,
 S, S f,
fibres and matrix. We note that, designating by I the length of the composite: vf _Sfl
v

Sl
V~
S m  m
_Sf
s
and that: S
~
The tensile stresses in the fibres and in the matrix are equal to:
0"/ =
E f s 1,
0"~ = Ems 1,
and the tensile force is given by:
Elastic constants of a unidirectional composite
F = S fo'f
47
+ SmtY~n .
The tensile stress cr I in the composite is" F
~'1     Vfo'! f "l" VmO"~ " (Vf E f "t" V m E m )E' l . S
The longitudinal Young's modulus E l of the composite is defined by: E l = tYl ~'1 and thus we obtain the relationship: E l =VfEf
+]/mE m = V f E f
+(lVf)em,
which provides a satisfactory value of E l . It should be noted that, for cases where E f >> E m , then as a first approximation: E l =VfEf.
3.4. Polsson' s coefficient v 12 With the loading described above the transverse extensions of the fibres and the matrix are equal to: Ef =  V f E I , E~ =VmE 1,
where v / and v m represent Poisson's coefficients of the fibres and the matrix. The change in thickness of the laminate is given by" Ae = Ae f + Ae m = e f e f + emE 2 ,
where e f and e m are the thicknesses of the fibre and matrix parts. Designating by 17the width of the composite, it may be noted that: v / ___ef b l _ e f Vf =
ebl
v
e
and: Vm mere e
.
The transverse expansion of the composite is: ~'2 =  e =
f f
9
48
Analysis of composite structures Poisson's coefficient Vl2 of the composite is defined by" t; 2 v12 =  ~ . El
From this we obtain the expression:
VI2  Vfvf
+ VmVm ' Vfvf "4 0 Vf )I/m,
which provides Poisson's coefficient VI2.
3.5. Transverse Y o u n g ' s modulus E 2
The composite is subjected to the transverse tensile force F. X2
matrix
I /
/
Xt
fibres FX 2 Figure 3.2. Transverse tension With the same model it is assumed that the transverse strains in the fibres and in the matrix are equal" 0"2 =0"2f =0.~n. The transverse extensions in the fibres and in the matrix are: _ 0"2 e.,f , 1_.
Ef
~.~n = 0"2 . Em The thickness variation is equal to:
Elastic constants of a unidirectional composite
49
Ae = Ae f + Ae m = e f e f + eme~' , the transverse extension of the composite is: =
e
= v:e
+ v,.c7
=
+
Ef
The transverse Young's modulus
E,n
.
E 2 of the composite is defined by the
expression:
1
c2
0"2 E2 from which we obtain" 1
E2
Ef
Em
The transverse Young's modulus E 2 is therefore equal to:
E2 =
EfEm
Em Em '
or~
Em
E2 =
lVf
Em )" l~f
The accuracy of the value of E 2 obtained by this expression is poorer than that for E l . When E f >> E m , the expression for E 2 becomes:
Em E2 = ~ .
lV/
From the calculations above it may be noted that the two Young's moduli E I and
E 2 are given by expressions analogous to those encountered when the
equivalent stiffnesses of two springs in parallel and in series are calculated.
3.6. Shear modulus G!2 The composite is subjected to shear loading 0"6 as shown on the following figure:
50
Analysisof composite structures
matrix
~
X
1
fibres
~//e~n ~
Figure
3.3.
6f
Shear
Again with the same model, it is assumed that the shear stresses in the fibres and in the matrix are equal" 0.6 =0.6f =0.~n. The angular distortions in the fibres and in the matrix are given by: Ef = 0"6 , Gf
~.~n = 0"6 , Gm
where G f and G m represent the shear moduli of the fibres and the matrix. The displacement in the Xl direction of the upper plane of the composite with respect to the lower plane is" u=uf
+um .
Given the displacements due to the fibre and matrix parts: Uf = e f E f , u m = emE ~ ,
we obtain: u
=
efEf6 + emE6m
=
[e, e.) Gf
+
Gm
0.6.
The angular distortion of the composite is: E6 = _
e
=
Gf
+
Gm
0" 6 ,
Elastic constants of a unidirectional composite
51
the Gl2 of the composite is given by"
1 = e6 GI2
9
0"6
SO:
_L=v:
.
G/
GI2
Gm
The shear modulus is: GI2 =
GfGm
Gm
VmG:+ V/G,. %+v: Gm c:
'
or: Gm
GI2 =
Once again the accuracy of Gi2 is less than that for E l . When Gf >> G m , we have, as a first approximation:
Gm lVf
GI2 = .
3.7. Longitudinal thermal expansion coefficient cq The composite is not subjected to any external force but experiences a temperature variation of:
AT=TTo. In the model considered here we assume that the longitudinal extensions of the fibres and of the matrix are identical, that is: eI =e(
=e~.
Only the longitudinal stresses due to the difference between the thermal coefficients of the fibres, a f and of the matrix a m are not zero. The longitudinal expansions of the fibres and the matrix are equal to: E/
e~n = o ' ~ + ~mAT" Em
52
Analysis of composite structures The longitudinal stresses in the fibres and the matrix are:
tr( = Ef (e,  ~ f A T ) , o'~n = Em (e I  t~mAT ). The resultant force of the tensile loads"
F=o'(Sf+o'~nSm, being zero, we obtain the expression"
V f o ' ( + VmO'~n = 0 . Introducing in this expression the stress values or[ and cry', we obtain:
V f E f (E1  o[,f AT)+ Vmg m (EI  O~'mAT)  O, then:
(Vf Ef + VmE m )El  (Vfo(,f E f + Vml~,mEm )AT . The coefficient of longitudinal thermal expansion
o~l of the composite being
defined by: 6"1 o~1  ~ , AT we obtain the following expression:
V f a f E / + VmamE m t~l

VfeI + V Em
VfafEf
+ (lVf)amE m
=
3.8. Transverse expansion coefficient
a 2
The transverse expansions of the fibres and matrix are equal to:
el2 = _ Vf o'( +otfAT, Ef m
e2 = 
Vm tr~ + OtmAT, Em
replacing the longitudinal stresses by their values determined in the previous paragraph we obtain:
ef = Vf(s l afAT)+afAT,
= Vm(e, a
Ar)+a
Ar.
The thickness variation is given by" Ae = Aef + Ae m = e f e f + eme ~ ,
Elastic constants of a unidirectional composite
53
The transverse expansion of the composite is" Ae ~ E2 ='=VfE +VmE ~. e Introducing the values of e~ and e ~ , we obtain:
E2
=
(Vfvf
+ VmV m )E l "6 (Vfolfl/f
"6 Vmt~mV m )AT Jr (Vfocf .6 Vmt~m ) A T .
As: el
=
V f a f E f + VmamE m
Vf E f "6VmE m
we have:
~' = {(~:~'
AT,
+"~176176176
..+ (VfGcfVf +VmOm l V+Vmfm m)(Vvff +Vmfm)}AT+(Vfocf +VmEm)AT ' or:
~ =[~,~m('..~, ~:~o)(~~~:) VI Ef
+ VINE.,
+ VfGCf .6 Vma m
]AT.
The coefficient of transverse thermal expansion a 2 of the composite given by: 0'2
s ="~,
is equal to: Ct2 = V f t~f + Vmt~ m +
VmE f  V f Em (Ctm _ Ctf ) Ef F E m
Vm Vf
or: t~2 " Vfot f
+(lV/)a m+ vmEEff lVf
 v f Em (Glm  tX.f ) + Em Vf
This Page Intentionally Left Blank
Chapter 4
Failure criteria 4.1. Introduction Having analysed the stresses and strains in composite materials we will now present the main failure criteria for these materials. The degradation of the composites is characterised by one of the following local modes:  damage dominated by fibre degradation (rupture, microbuckling, etc.),  damage dominated by matrix degradation (crazing, etc.),  damage dominated by singularities at the fibrematrix interface (crack propagation, delamination, etc.). Composite failure is a gradual process, as the damage in a layer results in a redistribution of stresses in the laminate.
4.2. Maximum stress theory Failure of the composite occurs as soon as the stress field no longer satisfies the following relationships: . . .
m
m
m
0.1rc < 0.1 < 0.1rt,
0.4r < 0"4 < 0.4r,
0.2rc < 0"2 < 0"2rt,
0.5r < 0"5 < 0.5r,
   .
~
m
0.3rc < 0"3 < 0.3rt,
,
.   ,
. . .
0.6r < 0"6 < 0.6r,
in which ~'irt (i = 1,2,3) represents the failure stresses in tension,
0.'irc (i = 1,2,3)
the
failure stresses in compression, and 0.'/r (i = 4,5,6) the shear failure stresses. In these expressions the failure stresses in tension and shear are positive, those in compression are negative. When the stress state in the composite is expressed as a function of a single parameter which depends on the external loads, it is convenient to introduce for each expression the loading coefficient Fit r associated with the stress state leading to failure.
56
Analysis of composite structures This stress state defined by:
~i = Fia~i (no summation), leads to the loading coefficients: !
Ft'tr = O'irt O"i
1
o r F itr = Orirc or i
(i = 1,2,3)
according to whether the normal stresses ~i are positive or negative and:
Fitr =O'i~r or Fitr=~ O"i
(i=4,5,6), O"i
according to whether the shear stresses ~i are positive or negative. Failure occurs for the smallest value of the loading coefficients Fit r , calculated above, according to the failure mode given by the index i. For i = 1, 2 or 3, failure occurs in tension or compression in the directions X l, X z or X 3 , whereas for i =4, 5 or 6, failure occurs by shearing in the planes (X 2, X 3 ), (X 3, X 1 ) or (X l , X z ).
4.3. Maximum strain theory Failure of the composite occurs as soon as the strain field no longer satisfies the following relationships: Eir c < E l < Elr t,
E4r < E 4 < E4r,
E2r c < E 2 < E 2 r t,
E5r < E 5 < E 5 r ,
E3r c < E 3 < E 3 r t,
E6r <E 6 <E6r,
in which Eitt (i = 1,2,3) represent the failure strains in tension, E"]rc ( i  1,2,3) the failure strains in compression and gir (i = 4,5,6) the shear failure strains. The failure strains in tension and shear are positive, whereas in compression they are negative. Just as for the maximum stress theory, if the strain state only depends on one parameter we can define for each expression the maximum strain coefficient Fie which is associated with the strain state leading to failure. This strain state: ~i' = F/e~i (no summation), gives the loading coefficients: Fie = Eirt
E2.
o r FiE " Eirc
(i = 1 , 2 , 3 ) ,
Failure criteria m
57
m
Fie =Eir or Fie =Eir (i=4,5,6) Ei Ei with, as for the maximum stress theory, the same remarks concerning the signs of the sign convention and the failure modes.
4.4. Polynomial failure criteria Composite failure occurs when the stress field no longer satisfies the expression:
FiN i + FijNiN j + Fukcritrjtr k + ... < 1
(i, j, k .... = 1, 2 ..... 6).
The coefficients F i , Fij and Fijk .... in this criterion are found experimentally. The different criteria described in the following paragraphs are of this type.
4.4.1. Tsai.HUl criterion The TsaiHill criterion is of the form'
Fij~i~j 0 a
a
the previous results become" 
for the displacements: ul = x 3 ~ ' J u2 = x3
Dtt + 2(Dr2 + 2D66)+ 322
u3 = ~)
 for the strains: El
Dll + 2(D12 + 2D66)+ D22
Dtt + 2(Dr2 + 2D66)+ D22
cos
/o)
sinsin
o
e2 =x3 ~
o
sin
a
sin nxl COS nx2 a a
Dl~ + 2(D~2 + 2D~)+ D22
~X 3
a
D~ + 2(D~2 + 2066)+ D22
a
a
sin n:r~ sin m 2 a
sin
mf I a
a
sin
Rx 2 a
Symmetrical orthotropic KirchhoffLove plates
a) e 6 = 2x 3 "~"

to" DI l + 2(D12 + 2D66)+ D22
COS
115
~1 ]Dr'2 ,,,COS a a
for the stresses:
0., = x3
(Q,, + Q,2 )D,, + 2(D,2 + 2 0 6 6 ) + 022
(0) 2
sin m~ sin/Dr a a
o'2 = x3 ~
tO' _sin n:x, sin m2.. ~ (Q,2 +Q21) D,, + 2(D,2 + 2D66)+ D22 o a
0"6 = 2x3
Q66 D, 1 + 2(3, 2 + 2 3 6 6 ) + 022
COS
a
COS~ , a
a (  ~ / 0"4 = ~ x~ 
m" s i n m t COS ~f2 " a a (Or2 + 2Q66 + 022 ) Dr, + 2(0,2 + 2 0 6 6 ) + 022
0"5 = " a~
(Q,2 + 2Q66 + Q , , ) D , , + 2(D,2 + 2D66)+ D22
X32 
cos
~fl /Dr2 sin a a
The maximum deflection at the centre of the plate is: u
~,
~
D,I +2(D, 2 + 2 D 6 6 ) + D22
It may be noted that u t, u 2, e I, e 2, e 6, 0.1' 0"2 and 0"6 vary linearly through the plate thickness, whereas u 3 is constant and o"4 and o"5 vary in a parabolic manner with the thickness. Also, u 3, e,, e 2, 0., and 0' 2 are zero around the edge, whereas u 2 and o"4 are zero for
xt=0, xl=aandx
x 2 =0, x 2=aand
2 = ~a.
We note that
u I and
o"5 are zero for
x I =~ and that e 6 and o"6 are zero for x I = ~  a n d x 2 = a
These conditions are illustrated in the following figures.  For the displacements:
~k
~
ul
x3
M0
k
."d U2
,
,
k
x3 M0
Mo u3
Figure 6.2. Variations in displacements
x3
116
Analysis of composite structures
x2
U1 = U3 = 0 .
.
.
.
.
.
.
a
: U2= 0 ..................................
2
~. ..................................
U 2 = U3 = 0
a 2
u2 = u3 = 0
u I =0
O uI = u3 = 0
x I
a
F i g u r e 6.3. Zero displacement
 For the strains:
El
"//]
M ~
i
E2
\ M ~
E6
F i g u r e 6.4. Strain variations
xzl
E l = E2 = 0
a
2
E6 = 0 ....................................................................
El = E 2 = 0 a
El = E 2 = 0
~e6 = 0
2 ,
O
!
E"1 = E 2 = 0 F i g u r e 6.5. Zero strain
a
x I
x3 M o
Symmetrical orthotropic KirchhoffLove plates  For the stresses: k
x3 Mo
0
0.1_
0"6
.....
Figure 6.6. Stress variations
x2
0.1 =0"2 = 0
1 !
a 2
,i 0"6 = 0 ..................................
I. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
0.1 =0"2 = 0 0.1 =0.2 = 0
a i0.6 = 0
5i
O
h~
0.1 =0"2 = 0
a
v
Xl
Figure 6.7. Zero stresses  For the transverse shear stresses"
t
~4
x3
! .......
x3
~'~4Z~
Figure 6.8. Transverse shear stress variations
117
118
Analysis of composite structures
x2~ 0"5 = 0
a
0' 4 = 0
2
a
0"4 = 0
o"4 = 0
0"5 = 0
2 0
0.5 = 0
a
v
xI
Figure 6.9. Zero transverse shear stresses
6.6. Free vibrations of a rectangular plate freely supported at its edge The free vibrations of a symmetrical orthotropic plate are governed by the equation:
0,, a,,,o ~i' + 2(o~ +2o66) ~x?~x~ a'u~ + o ~ a~u ~x~o + ~o ~a~.o : at 2
o"
The solution to this equation, which satisfies the boundary conditions around the edge in displacement and load:  f o r x I = 0 and x I = a l : u0 =0,
a2~
M 1 =Oil
a2~
aXl2 O12 ax 2 =0,
for x 2 = 0 and x 2 = a 2 9 u0 =0, M2 =  D l 2
U..~30 t~2 ~2uO =0, ax 2 D22
~x~
l
is of the form: uO =
3
Um,m2 sin
ml~l
al
sin
m2~'2
a2
sin(O)m,m2t+ (Pm,m2).
By introducing into the global vibration equation and after simplification by:
Symmetrical orthotropic KirchhoffLove plates sin m'~x' sin m2~2 sin(tOm,m2t + (Pmlm2),
al
a2
we obtain the equation: Di + 21mlitl ( m 2It 2 (D,2+2D66)...
miit
I
t , al ) t .
az
or: * 3 it 4 Dmim2 2 ) U mim2  [o(.Om,m2 = O,
with: * ml O'nim2 = al
DI I
" m2 (012 + 2066)+ m2 / 4 D22 , ~ "ml al ) ~ a2 )
+
a2 )
which provides the natural frequencies:
(m'l 4
o)
mira2
=It
2
~l
Dll
2 +
m_l al
2
m2 .
4
(DI2 + 2D66 )+ ~
.
.
.
Io
or'.
COmlm2 =
It2
Dmtm~ ]0
i ,, , The natural frequencies of a square plate of side a are given by'
I
m
O)mlm2 =
io
For a symmetrical orthotropic plate such that: DI 1 = 9D22, DI2 + 2 D ~ = 3D22, the natural frequencies are equal to: O)m l m 2
21 ' I0..... t
with:
k= ~/9m'~ +6m21m2 + m 4 = 3m 2 + m 2 .
a 2 ) ....
119
120
Analysis of composite structures For an isotropic plate, we have: (/)'mlm2 =
k'
Io
with: k'= m 2 + m
2 "
The influence of orthotropy on the order of appearance of the first four modes of vibration is shown in the table below: Orthotropic plate Mode
m2
1 1
1 2 3 1
l
1
2 3 4
ml
_.
2
4 7 12 13
.,
ml
Isotr0pic plate m2
k
1 1 2 2
1 2 1 2
2 5 5 8
9
Figure 6.10. Order of appearance of natural modes Its influence on the representation of the modes, and in particular the nodal lines (lines of zero transverse displacement), appears in the figure below: Mode
Orthotropic plate
lsotropic plate
+
+
i
+i
+
+

+ [i 
i+ Figure 6.11. Nodal lines
Symmetrical orthotropic KirchhoffLove plates
121
In the case of a symmetrical, orthotropic plate, it may be noted that the mode m I = l, m 2 = 3 appears before the mode m! = 2, m 2 = 2, the opposite order to that for an isotropic plate.
6.7. Buckling of a rectangular plate simply supported at its edge 6.7.1.
General case
The rectangular plate of transverse dimensions a I and a 2 is simply supported at its edge. It is loaded in compression  N O and  N O , with N~ > 0 and N O > 0 . N~
Ax3
a2
N~x2 N~ al
xI
II
Nt'x t Figure 6.12.
Buckling loads
The global buckling equation: tJ2M 1
t)2M 6
t)2M 2
igx~ +2oxlOxi ~ ~gx~
oO2U 0
N, ~x~ 
in which we have:
M,   o , , ax?  o,: axT' a2.o a2.o M 2 =  D r 2 0 x I2
O22~x2 '
0a2u~ N 2  ) x 2 = 0,
x2
122
Analysis of composite structures
M 6 =2D66
a2u~ ,
axl ax2
is written as:
Dll
a~u~ 2(o,, +
.ax41.+
a'~~ a~u~ No a'u~ 2D66)ax?ax 2.. +D22 a4~~ ax4 +N 0,ax2 + ax.~ = 0 . i
The boundary conditions for a simply supported plate are:  f o r x I = 0 and x I = a l : u0 =0,
a2~O M I =DII
a2~O
ax 2  D i E . a x
2
= 0,
forx 2=0and x2=a2: u 0 =0,
a2~O
a2.O
M 2 =  D I 2 ax,2. D22 ax22 =0. These conditions are satisfied by: u~ = U 3
mim2
sin ml/tXl sin m2/tx2 , aI
a2
which, after introduction into the global buckling equation and simplification, gives:
ml~ LL a,
Dl I +
2~ml~rl rm2~r ~
I t ai J It` a 2
(Di2 +2D66)+
_ 9
/
No_
al J
The critical buckling loads, corresponding to U 3
mi~r .
D22...
a2 m,~
a2
mira2
No
~
nonzero, are given by the
expression:
m/2.o a, j
a~ j
Lt a, )
m, m2] (D12+206~)+ m2 ...+ m, ta~ ~ ~D~, which in the particular case where N O = I N 0 , gives:
=0
mira2
Symmetricalorthotropic KirchhoffLoveplates
Np =~2 alJ '
~ml al
Oil+
123
~m2 (O12+2066)+ fm2/ D22 a2 1 , I I~2 ),'
(mll2+k(m212 t, al J a2 J
If, in addition the plate is square a I =a 2 = a, we have: No
+ 2D66)+ m4D22 = (_~)2 m~Dl, + 2m21m~(Dl2 m? +km~
We will now examine different special cases. 6.7.2.
Case of k=O
The plate is subjected to a compression load  N O in the x I direction. T X NI~
lllll/la,
al
,
x I

,
,,
,
x I
Figure 6.13. Compression loading in one direction
The critical buckling load is given by the expression: L[,a_~l )/4 Oil+ 2~ ml/2/m 2 12 (DII+2D66)+ (m 2 )4 D22 1 , Np = (/2[fmlnll/ral ~ [, al ) [, a2 [,'~2 ) or: NO
(=)2[(
= ~2
mla2 ~ al '
124
Analysis of composite structures For m 2 = l , this expression gives the series of curves plotted on the figure
below. For a given width a 2 and fixed values of m I and m 2 the value of the ratio aL a2
which cancels the derivative of the critical buckling load:
=[
m ralo]
is" l
a__Ll= ml ( D I I ) 4
a:
Nts~)
9
For this value, the critical buckling load is: 2
The critical buckling load thus obtained is independent of m I and its minimum value is found for m 2 = 1.
Np
mI = 1 m I =2 =3
O
.... ," al a 2
Filure 6.14. Critical buckling loads
The buckling of a plate loaded in compression in the x I direction occurs in such a way that there can be several halfwaves in the compression direction and only one in the perpendicular direction ( m E = 1 ). The critical buckling load is then given by the expression:
Np : ~
_ DII + 2(D12 + 2D66)+
a, )
and the minimum obtained for:
m,a~ )
D22
,
Symmetrical orthotropic KirchhoffLove plates
o,
~=m
125
1
l
r o,,/~
,,
is equal to:
NO :
E
(~/DIID22 + D, 2 + 2D66).
The intersection of the two plots of critical buckling load, relative to the two successive values m I and m I + 1, is found by equating: 2
[( )
NO =
mla2
l,,,I
aI
NO = l,,,t+t
DI 1 +2(D12 + 2 D 6 6 ) +
(ml + l)a 2 aI
(
o,
1
mla2
DI 1 + 2(D12 + 2D66)+
D22 ,
al 2 D22 ], (ml + l)a 2
which gives successively:
mla2 al
Di I +
=
rata2
D22 =
[(m I + 1)2 _ m 2 a__L D l l = al ) m2
( a ~ )4 = (m I + 1) 2 m  2D ~a 2 )
1 tn~
Di I +
al (m I + 1)
2
(ml + l)a 2
022,
D22'
1, ,
1 D22 (m I + 1) 2
or:
~,a2 )
~ D22
This expression enables the length a I to be calculated for a given value of a 2, for which the critical buckling load is identical for the modes m I and m I + 1. When a plate is subjected to a compression load  N o in the x I direction, the buckling of the plate occurs such that there exists:  in the x I direction: a single halfwave (m 2 = 1),  in the x2 direction: 1
 a halfwave for: 0
0.
Xl X3
" ""
Z
....."
0
O
Figure 11.2. By introducing the global loads:
Xl
Plateinbucklingsituation
226
Analysisof composite structures
dq/l
du o
N I=All__~t
+BII dx I '
aU~
N 2 = Al2 dx I ' au o
N6 = A 6 6 ~ , dxl
du o M l = B,,~+ a
D,,
d~l
t
dx~
dip" 1
M2 = Dl2 ~ , dx l M 6 =0, N 4 =0,
N5 = KA55 ~1 +

into the equations for global buckling: dNl =0, dXl dN6  0, dxl dMl dxl
N 5 =0,
dM6 dx l
N 4 =0,
dN5
N O d2u~ dx 2 = O,
dXl

we obtain the four equations: d2u~
d2~t =0,
All dx? +Bll dx~ d 2 u ~ _ O,
BII dx? + DII dx?  KA55 el + dx I j = 0,
Cylindrical flexure of multilayer ReissnerMindlin plates
d2u7 ) 
d~,! KA,,